#------------------------------------------------------------------------------
#$Date: 2016-02-11 02:03:02 +0200 (Thu, 11 Feb 2016) $
#$Revision: 176343 $
#$URL: svn://www.crystallography.net/cod/cif/2/10/35/2103501.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2103501
loop_
_publ_author_name
'Pavlovska, A.'
'Werner, S.'
'Maximov, B.'
'Mill, B.'
_publ_section_title
;
 Pressure-induced phase transitions of piezoelectric single crystals
 from the langasite family: La₃Nb~0.5~Ga~5.5~O₁₄ and
 La₃Ta~0.5~Ga~5.5~O₁₄
;
_journal_coden_ASTM              ASBSDK
_journal_coeditor_code           SN0021
_journal_coeditor_notes          ' ?'
_journal_date_accepted           2002-06-10
_journal_date_from_coeditor      2002-06-10
_journal_date_printers_first     2002-08-20
_journal_date_proofs_in          2002-10-30
_journal_date_proofs_out         2002-08-20
_journal_date_recd_electronic    2002-03-06
_journal_issue                   6
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              939
_journal_page_last               947
_journal_paper_category          FA
_journal_paper_doi               10.1107/S0108768102010273
_journal_techeditor_code         B021027
_journal_techeditor_notes
;
;
_journal_volume                  58
_journal_year                    2002
_chemical_formula_sum            'Ga5.54 La3 O14 Ta0.46'
_chemical_formula_weight         1110.22
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           150
_symmetry_space_group_name_Hall  'P 3 2"'
_symmetry_space_group_name_H-M   'P 3 2 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   8.213
_cell_length_b                   8.213
_cell_length_c                   5.115
_cell_measurement_temperature    293(2)
_cell_volume                     298.8
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_pressure         0.7E+6
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.704
_diffrn_measured_fraction_theta_max 0.704
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0765
_diffrn_reflns_av_sigmaI/netI    0.0453
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       5
_diffrn_reflns_limit_l_min       -5
_diffrn_reflns_number            1967
_diffrn_reflns_theta_full        27.94
_diffrn_reflns_theta_max         27.94
_diffrn_reflns_theta_min         2.86
_exptl_absorpt_coefficient_mu    27.018
_exptl_crystal_density_diffrn    6.170
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             488
_refine_diff_density_max         1.553
_refine_diff_density_min         -1.478
_refine_diff_density_rms         0.425
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   -0.10(5)
_refine_ls_extinction_coef       0.127(13)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   0.946
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     39
_refine_ls_number_reflns         367
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.946
_refine_ls_R_factor_all          0.0420
_refine_ls_R_factor_gt           0.0420
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1000P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0971
_refine_ls_wR_factor_ref         0.0971
_reflns_number_gt                367
_reflns_number_total             367
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            sn0021-0.7cad4.cif
_cod_data_source_block           0.7cad4
_cod_depositor_comments
;
The _diffrn_ambient_pressure was taken from the original data block
header, after comparison with the paper text and supplementary
material.

Saulius Gra\<zulis
;
_cod_database_code               2103501
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'y, x, -z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -x+y, -z'
'x-y, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
La La 0.42586(11) 0.0000 0.0000 0.0201(5) Uani 1 2 d S
Ga1 Ga 0.0000 0.0000 0.0000 0.0195(6) Uani 0.50 6 d SP
Ta Ta 0.0000 0.0000 0.0000 0.0195(6) Uani 0.50 6 d SP
Ga2 Ga 0.6667 0.3333 0.4687(6) 0.0189(7) Uani 1 3 d S
Ga3 Ga 0.7618(2) 0.0000 0.5000 0.0202(6) Uani 1 2 d S
O1 O 0.3333 -0.3333 0.176(4) 0.025(4) Uani 1 3 d S
O2 O 0.4518(14) 0.3056(16) 0.296(3) 0.033(3) Uani 1 1 d .
O3 O 0.2171(13) 0.0731(14) -0.243(2) 0.031(2) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
La La -0.2871 2.4523 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ta Ta -0.7052 6.5227 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ga Ga 0.2307 1.6083 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 La O3 67.6(5) . 6
O3 La O2 108.6(4) . 5_655
O3 La O2 140.7(4) 6 5_655
O3 La O2 140.7(4) . 3_655
O3 La O2 108.6(4) 6 3_655
O2 La O2 97.7(5) 5_655 3_655
O3 La O1 124.5(3) . .
O3 La O1 79.8(3) 6 .
O2 La O1 70.9(4) 5_655 .
O2 La O1 91.1(3) 3_655 .
O3 La O1 79.7(3) . 2_655
O3 La O1 124.5(3) 6 2_655
O2 La O1 91.1(3) 5_655 2_655
O2 La O1 70.9(4) 3_655 2_655
O1 La O1 153.00(8) . 2_655
O3 La O2 65.6(4) . 6
O3 La O2 78.8(4) 6 6
O2 La O2 65.5(4) 5_655 6
O2 La O2 153.72(17) 3_655 6
O1 La O2 64.9(4) . 6
O1 La O2 126.6(4) 2_655 6
O3 La O2 78.8(4) . .
O3 La O2 65.6(4) 6 .
O2 La O2 153.72(17) 5_655 .
O2 La O2 65.5(4) 3_655 .
O1 La O2 126.6(4) . .
O1 La O2 64.8(4) 2_655 .
O2 La O2 137.1(4) 6 .
O3 La Ga2 86.4(3) . 2_545
O3 La Ga2 111.0(3) 6 2_545
O2 La Ga2 32.2(2) 5_655 2_545
O2 La Ga2 127.8(2) 3_655 2_545
O1 La Ga2 64.6(4) . 2_545
O1 La Ga2 110.3(4) 2_655 2_545
O2 La Ga2 33.3(2) 6 2_545
O2 La Ga2 165.0(2) . 2_545
O3 La Ga2 111.0(3) . .
O3 La Ga2 86.4(3) 6 .
O2 La Ga2 127.8(2) 5_655 .
O2 La Ga2 32.2(2) 3_655 .
O1 La Ga2 110.3(4) . .
O1 La Ga2 64.6(4) 2_655 .
O2 La Ga2 165.0(2) 6 .
O2 La Ga2 33.3(2) . .
Ga2 La Ga2 159.53(3) 2_545 .
O3 La Ta 33.8(3) . .
O3 La Ta 33.8(3) 6 .
O2 La Ta 131.1(3) 5_655 .
O2 La Ta 131.1(3) 3_655 .
O1 La Ta 103.50(4) . .
O1 La Ta 103.50(4) 2_655 .
O2 La Ta 68.54(19) 6 .
O2 La Ta 68.54(19) . .
Ga2 La Ta 100.237(15) 2_545 .
Ga2 La Ta 100.237(15) . .
O3 La Ga1 33.8(3) . .
O3 La Ga1 33.8(3) 6 .
O2 La Ga1 131.1(3) 5_655 .
O2 La Ga1 131.1(3) 3_655 .
O1 La Ga1 103.50(4) . .
O1 La Ga1 103.50(4) 2_655 .
O2 La Ga1 68.54(19) 6 .
O2 La Ga1 68.54(19) . .
Ga2 La Ga1 100.237(15) 2_545 .
Ga2 La Ga1 100.237(15) . .
Ta La Ga1 0.0 . .
O3 Ga1 O3 163.3(6) 6 3
O3 Ga1 O3 107.0(6) 6 4
O3 Ga1 O3 85.5(4) 3 4
O3 Ga1 O3 84.5(6) 6 .
O3 Ga1 O3 85.5(4) 3 .
O3 Ga1 O3 85.5(4) 4 .
O3 Ga1 O3 85.5(4) 6 5
O3 Ga1 O3 107.0(6) 3 5
O3 Ga1 O3 84.5(6) 4 5
O3 Ga1 O3 163.3(6) . 5
O3 Ga1 O3 85.5(4) 6 2
O3 Ga1 O3 84.5(6) 3 2
O3 Ga1 O3 163.3(6) 4 2
O3 Ga1 O3 107.0(6) . 2
O3 Ga1 O3 85.5(4) 5 2
O3 Ga1 La 98.4(3) 6 4
O3 Ga1 La 98.4(3) 3 4
O3 Ga1 La 42.3(3) 4 4
O3 Ga1 La 126.5(3) . 4
O3 Ga1 La 42.3(3) 5 4
O3 Ga1 La 126.5(3) 2 4
O3 Ga1 La 126.5(3) 6 2
O3 Ga1 La 42.3(3) 3 2
O3 Ga1 La 126.5(3) 4 2
O3 Ga1 La 98.4(3) . 2
O3 Ga1 La 98.4(3) 5 2
O3 Ga1 La 42.3(3) 2 2
La Ga1 La 120.0 4 2
O3 Ga1 La 42.3(3) 6 .
O3 Ga1 La 126.5(3) 3 .
O3 Ga1 La 98.4(3) 4 .
O3 Ga1 La 42.3(3) . .
O3 Ga1 La 126.5(3) 5 .
O3 Ga1 La 98.4(3) 2 .
La Ga1 La 120.0 4 .
La Ga1 La 120.0 2 .
O3 Ta O3 163.3(6) 6 3
O3 Ta O3 107.0(6) 6 4
O3 Ta O3 85.5(4) 3 4
O3 Ta O3 84.5(6) 6 .
O3 Ta O3 85.5(4) 3 .
O3 Ta O3 85.5(4) 4 .
O3 Ta O3 85.5(4) 6 5
O3 Ta O3 107.0(6) 3 5
O3 Ta O3 84.5(6) 4 5
O3 Ta O3 163.3(6) . 5
O3 Ta O3 85.5(4) 6 2
O3 Ta O3 84.5(6) 3 2
O3 Ta O3 163.3(6) 4 2
O3 Ta O3 107.0(6) . 2
O3 Ta O3 85.5(4) 5 2
O3 Ta La 98.4(3) 6 4
O3 Ta La 98.4(3) 3 4
O3 Ta La 42.3(3) 4 4
O3 Ta La 126.5(3) . 4
O3 Ta La 42.3(3) 5 4
O3 Ta La 126.5(3) 2 4
O3 Ta La 126.5(3) 6 2
O3 Ta La 42.3(3) 3 2
O3 Ta La 126.5(3) 4 2
O3 Ta La 98.4(3) . 2
O3 Ta La 98.4(3) 5 2
O3 Ta La 42.3(3) 2 2
La Ta La 120.0 4 2
O3 Ta La 42.3(3) 6 .
O3 Ta La 126.5(3) 3 .
O3 Ta La 98.4(3) 4 .
O3 Ta La 42.3(3) . .
O3 Ta La 126.5(3) 5 .
O3 Ta La 98.4(3) 2 .
La Ta La 120.0 4 .
La Ta La 120.0 2 .
O1 Ga2 O2 118.0(4) 2_656 .
O1 Ga2 O2 118.0(4) 2_656 3_655
O2 Ga2 O2 99.8(5) . 3_655
O1 Ga2 O2 118.0(4) 2_656 4_665
O2 Ga2 O2 99.8(5) . 4_665
O2 Ga2 O2 99.8(5) 3_655 4_665
O1 Ga2 La 134.40(4) 2_656 .
O2 Ga2 La 56.2(4) . .
O2 Ga2 La 43.7(4) 3_655 .
O2 Ga2 La 107.2(4) 4_665 .
O1 Ga2 La 134.40(4) 2_656 2_655
O2 Ga2 La 107.2(4) . 2_655
O2 Ga2 La 56.2(4) 3_655 2_655
O2 Ga2 La 43.7(4) 4_665 2_655
La Ga2 La 76.45(6) . 2_655
O1 Ga2 La 134.40(4) 2_656 4_665
O2 Ga2 La 43.7(4) . 4_665
O2 Ga2 La 107.2(4) 3_655 4_665
O2 Ga2 La 56.2(4) 4_665 4_665
La Ga2 La 76.45(6) . 4_665
La Ga2 La 76.45(6) 2_655 4_665
O3 Ga3 O3 130.7(6) 5_655 3_656
O3 Ga3 O2 99.7(5) 5_655 3_655
O3 Ga3 O2 110.2(5) 3_656 3_655
O3 Ga3 O2 110.2(5) 5_655 5_656
O3 Ga3 O2 99.7(5) 3_656 5_656
O2 Ga3 O2 103.8(7) 3_655 5_656
Ga2 O1 La 110.2(4) 2_546 4_655
Ga2 O1 La 110.2(4) 2_546 .
La O1 La 108.7(4) 4_655 .
Ga2 O1 La 110.2(4) 2_546 2_545
La O1 La 108.7(4) 4_655 2_545
La O1 La 108.7(4) . 2_545
Ga3 O2 Ga2 117.3(7) 4_665 .
Ga3 O2 La 121.0(5) 4_665 4_665
Ga2 O2 La 104.1(5) . 4_665
Ga3 O2 La 113.0(5) 4_665 .
Ga2 O2 La 90.5(4) . .
La O2 La 106.4(5) 4_665 .
Ga3 O3 Ta 114.0(5) 4_664 .
Ga3 O3 Ga1 114.0(5) 4_664 .
Ta O3 Ga1 0.0 . .
Ga3 O3 La 137.2(5) 4_664 .
Ta O3 La 103.9(4) . .
Ga1 O3 La 103.9(4) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
La O3 2.424(9) .
La O3 2.424(9) 6
La O2 2.440(13) 5_655
La O2 2.440(13) 3_655
La O1 2.608(7) .
La O1 2.608(7) 2_655
La O2 2.847(12) 6
La O2 2.847(12) .
La Ga2 3.426(2) 2_545
La Ga2 3.426(2) .
La Ta 3.4976(9) .
La Ga1 3.4976(9) .
Ga1 O3 2.004(10) 6
Ga1 O3 2.004(10) 3
Ga1 O3 2.004(10) 4
Ga1 O3 2.004(10) .
Ga1 O3 2.004(10) 5
Ga1 O3 2.004(10) 2
Ga1 La 3.4976(9) 4
Ga1 La 3.4976(9) 2
Ta O3 2.004(10) 6
Ta O3 2.004(10) 3
Ta O3 2.004(10) 4
Ta O3 2.004(10) .
Ta O3 2.004(10) 5
Ta O3 2.004(10) 2
Ta La 3.4976(9) 4
Ta La 3.4976(9) 2
Ga2 O1 1.82(2) 2_656
Ga2 O2 1.882(10) .
Ga2 O2 1.882(10) 3_655
Ga2 O2 1.882(11) 4_665
Ga2 La 3.426(2) 2_655
Ga2 La 3.426(2) 4_665
Ga3 O3 1.833(10) 5_655
Ga3 O3 1.833(10) 3_656
Ga3 O2 1.871(11) 3_655
Ga3 O2 1.871(11) 5_656
O1 Ga2 1.82(2) 2_546
O1 La 2.608(7) 4_655
O1 La 2.608(7) 2_545
O2 Ga3 1.871(11) 4_665
O2 La 2.440(13) 4_665
O3 Ga3 1.833(10) 4_664
